HYDROXYAPATITE/POLYMER COMPOSITES FOR BONE REPLACEMENT
HYDROXYAPATITE/POLYMER COMPOSITES FOR BONE REPLACEMENT
Ter verkrijging van
de graad van doctor aan de Universiteit Twente, op gezag van de rector magnificus,
prof. dr. F.A. van Vught,
volgens het besluit van het College voor Promoties in het openbaar te verdedigen
op donderdag 15 Mei 1997 te 13.15 uur
geboren op 22 juni 1962
te Changzhi, Shanxi province, P.R. China
Dit proefschrift is goedgekeurd door:
Promotoren: Prof. dr. J. Feijen
Prof. dr. C.A. van Blitterswijk
Assistent promotor: Dr. ir. J.R. de Wijn
To Hongbo Our parents
CIP-GEGEVENS KONINKLIJKE BIBLIOTHEEK, DEN HAAG
Hydroxyapatite/polymer composites for bone replacement/
Qing Liu [S.l.:s.n.]
Proefschrift Universiteit Twente, Enschede, -met literatuur opgave.
Subject headings: Biomaterials / bone implants /polymers
A SEM photo shows the fracture surface of EMa-HA composite. Better contact between such EMa modified HA particles and polymer matrix can be seen.
© Q. Liu, Bilthoven, The Netherlands, 1997
All right reserved, No part of this document may be reproduced in any fashion by photostat, microfilm, or by any other means without permission of the publisher.
This thesis is based on the following publications:
1 Q. Liu, J.R. de Wijn and C.A. van Blitterswijk, "Composite biomaterials with chemical bonding between hydroxyapatite filler particles and PEG/PBT block copolymer matrix", (submitted to J. Biomed. Mater. Res.).
2 Q. Liu, J.R. de Wijn and C.A. van Blitterswijk, "A study on the grafting reaction of isocyanates with hydroxyapatite particles", (submitted to J. Biomed. Mater.
3 Q. Liu, J.R. de Wijn and C.A. van Blitterswijk, " Covalent bonding of PMMA, PBMA and poly(HEMA) to hydroxyapatite particles", (submitted to J. Biomed. Mater.
4 Q. Liu, J. R. de Wijn, C. A. van Blitterswijk, "Surface modification of nano-apatite by grafting organic polymers", (submitted to J. Biomed. Mater. Res.).
5 Q. Liu, J.R. de Wijn and C.A. van Blitterswijk, "Nano-apatite/polymer composites:
Mechanical and physicochemical characteristics", (submitted to Biomaterials).
6 Q. Liu, J.R. de Wijn, D. Bakker and C.A. van Blitterswijk, "Surface modification of hydroxyapatite to introduce interfacial bonding with PolyactiveTM 70/30 in a biodegradable composite", J. Mater. Sci.: Mater. in Med. 7:551-557, 1996
7 Q. Liu, J.R. de Wijn, C.A. van Blitterswijk, "Intermolecular Complexation Between PEG/PBT Block copolymer and Polyelectrolytes Polyacrylic Acid and Maleic Acid Copolymer", European Polymer J. (accepted)
8 Q. Liu, J. Weng, J. G. C. Wolke, C. A. van Blitterswijk, "A novel in vitro model to study the calcification of biomaterials" ( Submitted to Cells and Materials).
9 Q. Liu, J. R. de Wijn, D. Bakker, M. v. Toledo, C. A. van Blitterswijk, "Polyacids as bonding agents in hydroxyapatite/polyester-ether (PolyactiveTM 30/70) composites", (submitted to J. Mater. Sci. : Mater. in Med. )
10 J.R. de Wijn, Q. Liu and C.A. van Blitterswijk, "Grafting PMMA on hydroxyapatite powder particles using isocyanatoethylmethacrylate", Trans. Fifth World Biomaterials Congress, I-633 (May 29 -June 2, 1996, Toronto, Canada).
Chapter 1 General Introduction
Chapter 2 Surface modification of hydroxyapatite to introduce interfacial ...19
bonding with PolyactiveTM 70/30 in a biodegradable composite
Chapter 3 Polyacids as bonding agents in hydroxyapatite/polyester-ether ...33
(PolyactiveTM 30/70) composites
Chapter 4 Intermolecular complexation between PEG/PBT block copolymer ...47
and polyelectrolytes polyacrylic acid and maleic acid copolymer Chapter 5 Nano-apatite/polymer composites: Mechanical and
Chapter 6 A novel in vitro model to study the calcification ...73
Chapter 7 Surface modification of nano-apatite by grafting organic polymer ...85
Chapter 8 A study on the grafting reaction of isocyanates with ...97
Chapter 9 Covalent bonding of PMMA, PBMA and poly(HEMA) to ...113
Chapter 10 Composite biomaterials with chemical bonding between ...127
hydroxyapatite filler particles and PEG/PBT copolymer matrix
Chapter 11 General Discussion
General Introduction 1
1. Biomaterials for bone replacement
Much effort has been invested in the development of biomaterials for the repair or replacement of hard tissue. Besides the general consideration of biocompatibility, the specific consideration for bone replacement materials is of biomechanical nature: the biomaterials should possess the mechanical properties necessary for a proper performance in their function. Other properties such as biodegradation, the ability to bond to bone or so called "bone-bonding"
property are some additional favourable assets. The bone bonding property can be defined as [Williams et al. 1992]: "the establishment by physicochemical processes of a continuity between implant and bone matrix". Bone bonding properties - often called "bioactivity" - have been proved to be of great benefit for bone replacement materials.
1.1. Bone derived materials- autografts and allografts
The conventional method for the reconstruction of surgical osseous defects is dependent on an adequate supply of autogenous (host) or allogenic (donor) bone. Bone autograft is widely considered to be the best implant for repairing bone defects [Damien and Parsons 1991, Brown and Cruess 1982]. Common donor sites include the iliac crest, tibia, fibula and greater trochanter.
However, the amount of autogenous bone available for transplantation is limited, particularly in children. Also, the harvesting operation carries the risk of post-operative complications [Damien and Parsons 1991, Prolo and Rodrigo 1985]. Cortical bone is selected for strength and mechanical support, while cancellous bone autografts are used to promote lattice formation and rapid bone regeneration.
Allogenic bone has been successfully used in osseous reconstruction [Damien and Parsons 1991, Glowacki et al. 1981, Kaban et al, 1982] and offers several advantages over autogenous bone, including the avoidance of a harvesting operation, ease of manipulation and potentially unlimited material in bank form. Nevertheless, the possibility of transmission of disease from the donor to the recipient raises doubts about its future. Long times needed for the resorption and the replacement of allografts by new bone and the antigenic activity of banked bone are the serious disadvantages when compared with autografts. As a consequence, the search for suitable alternatives to autogenous and allogenic bone has intensified over the past decade.
1.2. Synthetic materials-metals, ceramics and polymers and composites 1.2.1. Metals
Metallic implants have been used either as permanent prostheses such as the hip prosthesis, dental implants, etc, or as temporary implants such as plates, pins, screws and rods
Chapter 1 2
for the fixation of bone fractures. Currently, stainless steel [Small and Misiek 1986], cobalt-chrome alloys [Albrektsson et al, 1986], Titanium and its alloys [Albrektsson et al, 1986, Steflik et al. 1993] have been used to fabricate the implants. These implants are usually not integrated by the bone tissue or only after extended implantation periods. Improvement of implant integration in bone can either be accomplished by cement fixation, the use of a porous bead implant surface to allow bone ingrowth and thus mechanical fixation or the application of bioactive ceramic coatings. Hydroxyapatite coatings applied by various methods [de Groot et al.
1987, Ducheyne et al. 1980, Lacefield 1988, van Raemdonck et al. 1984] are in clinical use today and improve implant performance. In some occasions, the high mechanical stiffness of metallic implants may result in stress-shielding and bone resorption due to the mismatch of elastic modulus of metals with that of bone [Daniels et al. 1990, Terjesen and Apalset 1988].
Other disadvantages of using metallic implants include the need for the second operation to remove temporary implants and the negative tissue response caused by the ions released from permanently implanted devices [Black 1981, Sinibaldik et al. 1976].
The use of ceramics can be dated back to 19th century when calcium sulphate (Plaster of Paris) was first used by Dreesmaanas as a plaster for the fixation of bone. Nowadays, the commonly used bioceramics are metallic oxides (e.g. Al2O3, MgO) [Black 1981], calcium phosphate (e.g. hydroxyapatite (HA), tricalcium phosphate (TCP), octacalcium phosphate (OCP)) [de Groot 1981, LeGeros, 1991], and glass ceramics ( e.g. Bioglass, Ceravital) [Hench et al.1971, Kokubo 1992]. The metallic oxides are considered to be nearly bioinert in biological environments, while calcium phosphate and glass ceramics can bond to bone in bony sites when implanted. Because of the good biocompatibility and bioactivity of the bioceramics, they have been successfully used for hard tissue replacement.
Among the bioactive ceramics, synthetic hydroxyapatite with a chemical composition Ca10(PO4)6(OH)2 has been extensively studied as a bone replacement material. As a bulk material, HA lacks sufficient tensile strength and is too brittle to be used in most load bearing applications [Denissen et al. 1980, Lemons 1988]. Therefore, when hydroxyapatite has to be applied in load bearing situations, the material is coated onto a metal core [de Groot et al.
1987], or is incorporated into polymers as composites [Bonfield et al. 1986, Doyle et al. 1991, Knowles et al. 1992, Verheyen et al. 1993].
Although polymers are widely used as implants, such as vascular prostheses, sutures etc.
only limited number of polymers have been used for bone replacement purposes due to the limitation of their mechanical properties. These polymers include ultra-high molecular weight polyethylene (UHMWPE)[Park and Lakes 1992], poly(methyl methacrylate) (PMMA)[Saha and
General Introduction 3 Pal 1984, Pilliar et al 1976], polylactide (PLA), polyglycolide (PGA) and polyhydroxybutyrate [Daniels et al. 1990, Knowles et al. 1992, Coombes and Meikle 1994, Agrawal et al. 1995].
The choice of polymer as bone replacement material largely depends on the following factors (besides the general requirement of biocompatibility): (1). The mechanical properties of the polymer if the polymer is going to be used as load bearing material; (2). The biodegradation behaviour of the polymer if the implant has to be eliminated after certain period. (3). The ability to bond with bone or to induce bone ingrowth.
Generally speaking, polymers have poorer mechanical properties than bone. But the possibility to be mechanically strengthened and to be biodegradable makes polymers very promising as candidates for bone replacement. The improvement of the mechanical properties of polymer can be achieved by either the modification of the structure of the polymer, or the strengthening of the polymer with fibre and/or filler as it will be discussed later.
The structure modification of polymers includes crosslinking, copolymerization more than one type of monomer, using new type of monomers to synthesize new polymers, etc. Some researchers have synthesized polyimminocarbonates by incorporating tyrosine, tyroamine or desamino-tyrosine groups to the polymer chain [Pulapura et al. 1990, 1992]. They found that the synthesized poly(desaminotyrosyl-tyrosine hexylester iminocarbonate) had a tensile strength of 40 MPa, and a tensile modulus of 1.6 GPa which is relatively high among the biodegradable polymers. Attawia et al  incorporated aromatic imide groups to poly(anhydrides) to improve the mechanical properties of poly(anhydrides).
Although the biodegradation ability of the polymer can be carefully designed by introducing ester bonds, imino bonds etc. to the polymer structure, it is rather difficult to obtain a polymer both biodegradable and mechanically strong to the level of cortical bone.
Poly(lactide)( PLA) and poly(glycolic acid, PGA) seem still to be the strongest biodegradable polymers available for medical applications; they can have a tensile strength up to 72 MPa for PLLA, 57 MPa for PGA and a Young's modulus of 4 GPa for PLLA and 6.5 GPa for PGA [Daniels et al. 1990]. Compared with the mechanical properties of cortical bone, these polymers are still weaker and reinforcement of the materials is still necessary.
The bone bonding property of a polymer is another issue of concern. Up to now, only a polyethylene/polybutylene terephthalate (PEG/PBT) block copolymer (PolyactiveTM) has been identified as a "bone bonding polymer" [Bakker et al. 1989, 1990a, 1990b, 1990c, van Blitterswijk et al, 1993a]. It is explained that the PEG segments of the material can complex calcium ions and thus cause calcification of the polymer. The calcification of the polymer is believed to be a prerequisite for the following bone-bonding to occur [van Blitterswijk et al.
1992]. Although some other polymers were also found to be calcified in vivo, such as polyetherurethane [Coleman 1981, Wisman et al.1982, Schoen et al 1988, Thoma 1987] or poly(HEMA) hydrogel [Swart 1976], none of the above polymers has been studied for bone bonding properties.
Chapter 1 4
The design of polymers with bone-bonding property has not been progressed very much.
Since the calcification of material is the common feature shared by bone-bonding biomaterials such as Bioglass [Hench et al. 1971, 1981], AW glass ceramics [Kokubo et al. 1990, 1991, 1993], hydroxyapatite [Jarcho 1981, LeGeros et al. 1992, Ducheyne and Cuckler 1992, van Blitterswijk 1995], and PEG/PBT block copolymer [van Blitterswijk et al. 1992, Radder et al.
1993], the introduction of certain functional groups to the polymer chain or the surface may give the polymer the ability to induce calcification and thus to have bone-bonding abilities.
Dalas et al [1991a, 1991b] have shown that introduction of functional groups like the phosphinyl group, the carboxylic acid group, the sulphonate group, fluoride et al, may induce the nucleation of hydroxyapatite on the polymer. Tretinnikov et al  showed that introduction of phosphate groups to the surface of high density polyethylene can induce the formation of a firmly bonded carbonated apatite layer on the surface upon immersion in simulated physiologic solution. When the surface modified polyethylene rod was implanted in the rat femur, they found a high percentage of bone contact for the experimental samples as compared to the control untreated polyethylene rod [Kamei et al. 1996]. Li et al [1996, 1997a, 1997b, 1997c] modified natural bamboo by various methods, including grafting of PEG and introduction of phosphate groups to cellulose of bamboo. The modified bamboo has the ability to induce apatite formation in vitro.
1.2.4. Polymer Matrix Composites
The use of polymer matrix composites for bone replacement may offer the advantages of avoiding the problem of stress shielding, eliminating the need for a second surgical procedure to remove the implants if the implants can be made biodegradable and also the elimination of the ion release problem of metal implants. The possibility to make the composites as strong as cortical bone and to improve the material's bioactivity or bone bonding activity by adding of a secondary reinforcing phase makes the composites very attractive. Fibers and mineral filler particles have been used to reinforce the polymer materials as well as to improve the bone-bonding properties of the composites.
2. Polymer Matrix Composite
2.1. Fiber reinforced composites (FRC)
Carbon fiber, aramid (Kevelar), glass fiber, usually posses very high strength and stiffness [Hancox 1983] and therefore have been frequently used to reinforce polymers like epoxy resin, polyetheretherketone (PEEK), polysulfone (PS), polymethyl methacrylate (PMMA), poly(lactide), poly(glycolide), polycaprolactone, etc. (table 1).
By proper choice of the type of polymer matrix and of the fiber, the composites can be made totally biodegradable [Casper et al. 1985, Kelly et al. 1987, 1988, Andriano and Daniels 1992a,1992b, ], partially degradable [Zimmerman et al. 1987], or non-biodegradable [Latour
General Introduction 5 and Black 1992, 1993]. Also the mechanical properties can be tailored by combining different polymer matrices and fibers. As an example, 30 % carbon fiber reinforced PEEK composites has an elastic modulus of 17 GPa ( bone 7 -20 GPa), a flexural strength of 320 MPa (bone 150-250 MPa) [Hastings et al. 1987].
Bone bonding can be improved by using certain bioactive fibers. Marcolongo et al.
[1995, 1996] showed that when bioactive glass reinforced polysulfone composites were implanted for 6 weeks, direct apposition of bone tissue with bioactive glass fibers could be observed. Bone tissue was also observed in direct apposition to polymers surrounding the glass fibers.
When making fiber reinforced composites, the mechanical properties of the polymer matrix and the fiber are certainly important for the mechanical properties of the composites.
However, the interfacial bonding strength between fibers and polymer matrix is usually weaker than the polymer matrix [Pigott et al. 1985]. Therefore the fatigue fractures usually occur at the interface of fiber and polymer.
Table 1. Examples of fiber reinforced composites for bone replacement Carbon fiber
Epoxy resin [Bradley 1980, Tatton et al. 1982]
PMMA [Schreiber 1971, Wylegala 1973, Pilliar et al 1976, Ekstrand et al 1987]
polysulfone [Huettner et al. 1984, Claes et al 1986, Wenz et al.1990, Latour and Black
polycarbonate [[Latour and Black 1992]
polyetheretherketone [Hastings et al. 1987, William et al. 1987,Wenz et al.1990]
Polylactide [Zimmerman et al. 1987, Alexander et al. 1981]
PMMA [Berrong et al. 1990, Pourdeyhimi et al, 1986]
polysulfone [Latour and Black 1992, 1993]
polycarbonate [[Latour and Black 1992]
Polyethylene fiber (high-performance)
PMMA [Cheng et al, 1993], poly(DL-lactic acid [Fenner et al. 1996]
Bioactive glass fiber
polysulfone [Marcolongo et al. 1995, 1996]
Calcium metaphosphate glass fiber
polylactide [Casper et al. 1985, Kelly et al. 1987, 1988]
Calcium phosphate glass fiber
poly(L-lactide) [Lin, 1986], polycaprolactone [Foy et al.1996], poly-(desamino-tyrosyl-tyrosine ethyl ester) [Perez et al. 1996]
Calcium-sodium-metaphosphate glass fiber
Chapter 1 6
Poly(ortho ester) [Andriano and Daniels, 1992a,b]
PMMA [Topoleski and Ducheyne 1992]
When the composite is exposed to an in vivo environment, the interface of fiber and polymer can be further deteriorated. Several studies have shown the effect of water and simulated in vivo environments on the interfacial bonding strength of ceramic or glass fiber and polymer [ Ekstrand, et al. 1987, Foy et al. 1996, Latour and Black, 1992, 1993, Kelly at al. 1988, Andriano et al,1992a, 1992b, Jancar at al. 1993, Slivika et al. 1996]. There is clearly a need for the improvement of the interface of fiber/polymer matrix to improve both the mechanical properties of the composites and the wet stability of the interfacial bond.
2.2. Filler Reinforced Composites
The use of particulate fillers to reinforce polymeric biomaterials is quite important and quite successful in clinical applications, like dental restorative resins and bone cement [Soltese, 1988].
The purpose of using filler particles in the polymer matrix is to improve the mechanical properties such as the elastic modulus [Guida et al. 1984, Castaldini et al. 1984, Bonfield et al.
1984, 1986], fatigue behaviour [Castaldini et al. 1987] and to improve the bioactivity or bone-bonding properties [Bonfield et al. 1986, Doyle et al. 1991, Knowles et al. 1992, Verheyen et al. 1993]. Some other benefits may also obtained by using fillers, such as to diminish the creep of the composites [Castaldini et al. 1986] and to decrease the temperature rise during the polymerization of bone cements [Guida et al. 1984].
The use of a bioactive filler such as hydroxyapatite (HA), AW ceramic or Bioglass particles to reinforce a polymer may improve both the mechanical properties and the bone bonding properties. As indicated by Bonfield et al [1983, 1986, 1988], the elastic modulus of polyethylene can be increased from 1 GPa to about 8 GPa, which is in the low band of the value for bone, retaining a fracture toughness comparable to bone. When implanted in vivo, the HA/PE composites can induce bone apposition and thus create a secure bond between the natural bone and the implant. Inspired by this work, researches have been extended to the biodegradable polymer matrix. When implanted in vivo, such composites will induce bone formation or bone ingrowth and as the biodegradable polymer matrix degrades the implant will finally be replaced by bone tissue. The load thus can be gradually transferred to the newly formed bone. Based upon this idea, several hydroxyapatite reinforced biodegradable polymer composites have been developed, such as HA/polyhydroxybutyrate [Doyle et al, Knowles et al.
1991, 1992, Boeree et al. 1993], HA/polylactide [Verheyen et al. 1992,1993].
The use of a filler to reinforce a biodegradable polymer matrix offers another advantage:
General Introduction 7 the possibility to control the biodegradation rate. It has been shown that by addition of basic fillers, such as HA and magnesium oxide, the degradation rate as well as the degradation mechanism of poly (DL-lactide) can be changed [van der Meer et al.1996] Jones and Williams  also showed that the degradation pattern of poly(L-lactide ) was affected by the addition of ceramic filler.
Although the mechanical properties of the composites can be improved to a certain extent by the addition of bioactive filler particles, it is stated by several researchers [Verheyen et al.
1992, Wang et al.1994] that there is still a need to improve the bonding between filler and matrix since there is clearly no other bonding force between the two phases than mechanical interlock.
The use of certain coupling agents was suggested [Verheyen et al. 1992, Wang et al 1994].
3. Method to improve the interfacial bonding of the phases in composites 3.1. Self-reinforcement of fiber/polymer composites (SRC)
Polymer fibers usually possess much better mechanical properties, due to the molecular orientation, when compared to its bulk materials. Use of polymer fibers to reinforce a polymer matrix of the same chemical structure thus will result in a composite without a real interface between fibers and polymer matrix. Such self-reinforced composites have been made by using PLA [Vainionpaa et al. 1988], PGA [Laiho et al. 1988, Pellinen et al. 1988] and PMMA [Gilbert et al. 1995]. The mechanical properties of the composites were significantly improved by using this method. However, the polymer fibers used are still pliable, therefore the Young's modulus of SRC's can not be as high as the glass fiber and carbon fiber reinforced composites. On the other hand, the bone bonding properties of the composites can not be improved by this method.
3.2. Plasma treatment of fibers
Gas plasma treatment has been proven to be effective in enhancing the bond strength between fibers and polymer matrix. The gas used for the treatment of fiber can be argon gas, O2, methane or CO2 [Friis et al. 1996, Perez et al. 1996, Hild and Schwartz]. These methods have been used to treat fibers like polyethylene, calcium phosphate glass fiber and PET (table 2)
Table 2. Examples of using gas plasma treatment for the improvement of fiber/matrix interface
Fiber Gas Matrix
air poly(DL-lactic acid) [Fenner et al. 1996]
N2, Ar, CO2, PMMA [Hild et al. 1996]
PET Ar, O2, PMMA [Friis et al, 1996]
Chapter 1 8
Calcium-phosphate glass fiber
CH4 poly(DTE carbonate) [Perez et al. 1996]
During the gas plasma treatment, functional groups are generated on the surface of the fiber, therefore the wettability of the fibers by the polymer matrix and thus the bond strength between them is improved.
3.3. Silane coupling agents
A coupling agent is an additive which promotes the development of a strong bond between the filler(fiber) surface and the polymer. Silane coupling agents have been widely used to improve the bonding strength of the two phases and have a general formula as:
X represents a hydrolysable group, Y is a organofunctional group. The organofunctional groups are chosen for reactivity or compatibility with the polymer, while the hydrolysable groups are merely intermediate in the formation of a bond with the filler or fiber surface. The exact behaviour of coupling agent is a matter of some controversy.
The use of coupling agent has two purposes. The first one is to improve the mechanical properties of composites by improving the interfacial bonding strength. The second one is to prevent the surface dissolution of fibers. When using the silane coupling agent [3-(n-styrylmethyl-2-aminoethylamino)-propyltrimethoxysilane hydrochloride] to make calcium phosphate glass fibers reinforced polycaprolactone composites [Foy et al. 1996], the ultimate bond strength was improved both in dry and wet environments, but the ultimate bond strength remained still far below desirable working levels. Andriano et al [1992a, 1992b] used N, beta-aminoethyl-gamma-aminopropyl-trimethoxysilane to treat the surface of calcium-sodium-metaphosphate (CSM) mineral microfibers, which were used to reinforce poly(ortho esters) prepared by a condensation reaction of 3,9-bis(ethylene 2,4,8,10-tetraoxaspiro[5,5]-undecane) and a 60:40 and 90:10 mole ratio of flexible diol, 1,6-hexanediol, respectively. The choice of such a diamine silane coupling agent was also intended to neutralize the CSM fiber's acidity which may cause a fast degradation of the composites. The initial mechanical properties of the composites were modestly improved, and the wet resistance of the composites during in vitro exposure to Tris-buffered saline was markedly improved .
Other research showed that the use of silane coupling agents may still offer hydrolytic problems of the interface. Jancar et al  used 4 types of silane coupling agents to treat the E-glass fibers: amino-propyltriethoxylsilane, glycidoxy propyltrethyoxysilane, methacryloxypropyltrethoxy-silane, amiophenyltriethoxysilane. Although an improved adhesion was observed for some composites, the coupling agents did not prevent the deterioration of the interface under extreme conditions of stress and moisture (100 hrs, 85 oC in water). Applying a
General Introduction 9 silane layer by plasma polymerization on PET fiber surface did not change the fracture toughness of bone cement [Friis, et al. 1996].
In all these cases, it was noted that silane coupling agents did not form covalent bonds with the polymer matrix. The interface improvement is most probably due to the result of better wetting of the fiber surface by the polymer matrix.
The use of silane coupling agents in mineral filled dental resins has been employed since the 1960's [Bowen 1963, Venhoven 1994, Jones and Rizkalla 1996] as a method to improve the bonding of the filler to the resin. It was reported that appropriate silane coupling agents were chosen for a variety of mineral fillers to improve the mechanical properties of composites [Pluedemann 1991]. The greatest improvement was observed with silica, alumina, glass, silicon carbide, and aluminum needles. A good but somewhat lesser response was observed with talc, wollastonite, iron powder, clay, and hydrated aluminum oxide, only a slight improvement was imparted to asbestine, hydroxyapatite, titanium dioxide, and zinc oxide.
Surfaces that showed little or no apparent response to silane coupling agents included calcium carbonate, graphite and boron. Those results suggest that the coupling activity of silanes is not universal to all mineral surfaces.
The latest results showed that silane [3-trimethoxysilyl)-propyl methacrylate](MPS) treated glass filler can drastically decrease wear rates [Venhoven et al. 1994] in a dental resin based on BisGMA systems. Also, Jones et al  reported that a silane treated bioactive glass filler was found to have a significant effect on the elastic modulus of Bis-GMA based composites. Generally speaking, silane treated glass-ceramic, quartz, or silica particles may have a positive effect on the strength, stiffness and wear resistance and other aspects of the composites [Soltesz 1988, Chowdhury et al. 1995].
The effect of the use of silane coupling agents on hydroxyapatite (HA) seems to have somewhat controversary results. It has been shown that silane treated HA particles have a positive effect on the mechanical properties of a composite. Behiri et al  showed that applying methacryloxypropyltrimethoxysilane (MPS) to the surface of HA particles may enhance the tensile modulus, yield stress and elongation to fracture of polyethylmethacrylate cements. Labella et al  found that by using MPS, the hardness, flexural strength and diametral tensile strength of dental composites were significantly improved.
However, silane coupling agents also have been found to have different effect on the mechanical properties of other composites. Deb et al  and Nazhat et al  showed that MPS treated HA showed decreased tensile strength and Young's modulus of polyethylene composite. Since in both cases there was no chemical bonding between the silane and the polymer matrix, the decreased strength and modulus was explained by a plasticizing effect of the coupling agent. Surface treatment of β-crystalline metaphosphate with silane coupling agent MPS did not have effect on the tensile strength of dental resin composites [Antonucci et al.
Chapter 1 10
In our opinion, the different results of silane treatment probably depend on the covalent bonding between the silane coupling agent and the polymer matrix. Once a bonding was established between HA and silane, the bonding between silane coupling agent and polymer matrix did determine the interfacial strengths. In dental resin systems, when MPS was used, double bonds were introduced by the treatment of filler. In the following curing process, the bound MPS copolymerized with Bis-GMA monomer, so that a chemical linkage was introduced, and the mechanical properties were improved. In the use of HA/PE system, the introducing of MPS can not lead to a chemical bonding between MPS and PE matrix, therefore no improvement can be observed.
Apparently more efforts should be put in the selection of right silane coupling agents for different polymer matrix. Also, the effect of silane coupling agents on the bioactivity of HA particles has to be studied. Dupraz et al  studied different silane coupling agents on HA powder and showed by a XPS study that a few monolayers of silane film were present on the surface of HA particles. The silane thin film was "transparent" for ionic transport, although aminosilane coatings delayed the release of calcium and phosphate ions during the first few days of immersion of the treated HA powders in Gomori's buffer. In this sense, the bioactivity of the HA particle might be affected by the silane treatment, because the dissolution behaviour of HA plays an important role in its bone bonding activity [LeGeros et al. 1992,van Blitterswijk et al.1995].
3.4. Other methods
Ishhara et al [1989, 1992] found that 4-methacryloyloxyethyl trimellitic anhydride (4-META) containing MMA bone cement could adhere to bone, metals, HA and a composite of HA and fluoroapatite (FAP) with a improved tensile bond strength. The bonding of such cement to dentin was explained by the ability of 4-META to promote the interpenetration of monomers into dentin tissue. No explanation was given to the adhesiveness of such cements to HA and metals. We speculate that the formation of 4-methacryloyloxyethyl trimellitic acid (4-MET) was the reason of adhesion to HA. According to the authors [Ishhara et al. 1989], the anhydride moiety of 4-META can be easily converted to 4-MET by the reaction with water, thus the real mechanism might either be that 4-MET is firmly absorbed to the surface of HA followed by the copolymerization of 4-MET with MMA monomer, or the copolymerization takes place first and is followed by the adsorption of 4-MET moieties onto HA. In both cases, the interface of HA and polymer may be improved.
Misra  found that when the HA surface had been surface treated with zirconyl methacrylate, the diametral tensile strength of dental composites was increased by 50%.
Antonucci et al  also found that treatment of fillers by zirconyl methacrylate resulted in a modest enhancement of the tensile strength of the experimental composites.
Introduction of covalently bonded hydroxyethylmethacrylate (HEMA) to a
General Introduction 11 nonstoichiometric apatitic calcium phosphate was realized by a co-precipitation of apatitic octacalcium phosphate (AOCP) in the presence of hydroxyethylmethacrylate phosphate [Delpech and Lebugle 1990, Dandurand et al. 1990]. The bond of the organic HEMA to AOCP was realized by the ionized phosphate groups which partially replace the OH- ions located at the tunnel end in the apatite crystal structure. The obtained so called phosphoHEMA apatite then can be used to copolymerize with either HEMA or methyl methacrylate (MMA) to form chemical bonds between the mineral filler and the polymer matrix. It is claimed that such filler could stiffen the PMMA bone cement.
3.5. The nature of the bonding between silane coupling agent and hydroxyapatite
Although silane coupling agents have been used for the surface treatment of calcium phosphate mineral fibers or filler particles, the actual nature of the bond between silanes and the hydroxyapatite is still not clear. For the reaction of silanes with other minerals, two possible mechanisms may be involved in the treatment [Plueddemann 1991].
Due to absorption (hydrogen bonding), all the minerals and metal oxides are covered with at least a monolayer of water at ambient conditions. Alkoxysilanes are capable of reacting with surface moisture to generate silanol groups which also may form strong hydrogen bonds with the hydroxylated surface. This mechanism was supported by experiment [Nishiyama et al.
1987]. A chemical bonding mechanism presumes that water is adsorbed on the nonhygroscopic oxides as hydroxyl groups; Alkoxysilanes are capable of reacting with surface hydroxyl groups to form covalent oxane bonds with the mineral surface .
As for HA, little work has been done except for the work done by Nishizawa et al .
They used silane coupling agents to treat calcium phosphate ceramics. By using thermal analysis, infra-red and mass spectra, they found that the surface hydroxy groups of the ceramics formed covalent bonds with silane coupling agents.
4. PEG/PBT copolymer (PolyactiveTM)
The bone-bonding properties of poly(ethylene glycol)/poly(butylene terephthalate) (PEG/PBT) block copolymers was first reported by Bakker et al [1989, 1990a, 1990b, 1990c]. It has been found that when the PEG/PBT ratio is higher than 55/45, the copolymer has bone-bonding properties. By varying the ratio of PEG and PBT, as well as the molecular weight of PEG, a series of PEG/PBT copolymers can be synthesized with different mechanical properties, as well as different biological characteristics [van Blitterswijk et al. 1992, 1993, Radder et al. 1994], such as biodegradation rate and bone bonding properties. Concerning the bone-bonding property, it has been proposed [van Blitterswijk et al. 1992, 1993] that the PEG segment of polyactive can complex calcium ions from the environment by a similar mechanism proposed for the calcification of polyetherurethane [Thoma 1987]. The calcification in
Chapter 1 12
PolyactiveTM is at least composed of carbonated apatite, and thus similar to the apatite layer formed on other bioactive ceramics and to the mineral phase of bone [Radder et al 1993]. It is hypothesized that following calcification of the PEO/PBT copolymer surface, bone apposition can take place in a similar manner as on the surface apatite layer of other bioactive biomaterials which initially contain calcium and phosphorus ions.
Since the bonding of bone to Polyactive only occurs after the calcification of the polymer, Gaillard  used bioactive fillers like HA and AW glass particles to accelerate the calcification process of PolyactiveTM, and to promote the bone formation on the implant surface.
It was found that the in vitro calcification of both composites was increased by adding AW glass and HA filler particles. Also by precalcification of PolyactiveTM, the bone bonding rate of the materials can be accelerated [Gaillard et al. 1994].
5. Objective and methods
The objective of this study is to develop a suitable method to improve the interface of hydroxyapatite filler particles/PolyactiveTM composites. As we discussed before, the interface of filler and polymer plays an important role in determining the ultimate mechanical properties of composites.
Two methods were developed to improve the interface of HA and /PolyactiveTM. The first method is to introduce hydrogen bond interaction and/or ionic dipole interaction between the filler and polymer matrix by pretreatment of HA filler particles with polyacrylic acid and ethylene-maleic acid copolymer.
The second method was to introduce covalent bonding between HA and the polymer matrix by using isocyanate group containing coupling agents to graft the same polymers as the matrix to the particle surface. An acrylic resin system was chosen as a model system for the purpose. Also, PolyactiveTM 70/30 was grafted to the surface of HA via hexamethylene diisocyanate.
1 T. Albrektsson, G. Zarb, P. Worthington, A.S. Ericsson, "The long-term efficacy of currently used dental implants: A review and proposed criteria of success," Int. J. Oral Maxillof. Impl., 1,11-25, (1986).
2 H. Alexander, N. Langrana, J.B. Massengill, A.B. Weiss, "Development of new methods for phalangeal fracture fixation," J. Biomech., 14, 377-387 (1981).
3 K.P. Andriano, A.U. Daniels, "Biocompatibility and mechanical properties of a totally absorbable material for orthopaedic fixation devices," J. Appl. Biomater., 3,197-206, (1992a).
General Introduction 13 4 K.P. Andriano, A.U. Daniels, "Effectiveness of silane treatment on absorbable
microfibers," J. Appl. Biomater., 3, 191-195, (1992b).
5 J.M. Antonucci, B.O. Fowler, S. Venz, "Filler systems based on calcium metaphosphates," Dent. Mater., 7, 124-129 (1991).
6 M.A. Attawia, K.E. Uhrich, E. Botchwey, M. Fan, R. Langer, C.T. Laurencin,"
Cytotoxicity testing of poly(anhydride-co-imides) for orthopaedic applications," J.
Biomed. Mater. Res., 29, 1233-1240 (1995).
7 D. Bakker, J.R. de Wijn, C.M.F. Vrouwenraets, S.C. Hesseling, J.J. Grote, C.A. van Blitterswijk, "The reactions of bone to Polyactive, a bone-bonding copolyetherester," in Polymers in Medicine and Surgery, pp.11-15, (1989).
8 D. Bakker, C.A. van Blitterswijk, S.C. Hesseling, H.K. Koerten, W. Kuijpers, J.J. Grote,
" Biocompatibilty of a polyether urethane, polypropylene oxide, and a polyether polyester copolymer. A qualitative and quatitative study of three alloplastic tympanic membrane materials in rat middle ear," J. Biomed. Mater. Res., 24,489-515, (1990a).
9 D. Bakker, C.A. van Blitterswijk, S.C. Hesseling, W.T. Daems, J.J. Grote,
"Tissue/biomaterial interface characteristics of four elastomers. A transmission electron microscopical study," J. Biomed. mater. Res. 24, 277-293, (1990b).
10 D. Bakker, J.J. Grote, C.M.F. Vrouwenraets, S.C. Hesseling, J.R. de Wijn, C.A. van Blitterswijk, "Bone-bonding polymer (PolyactiveTM)," in Clinical Implant Materials, Advances in Biomaterials 9, pp.94-104, (1990c).
11 J.C. Behiri, M. Braden, S.N. Khorasani, D. Wiwattanadate, W. Bonfield, "Advanced bone cement for long term orthopaedic implantations," Bioceramics, 4, 301-307 (1991) 12 J.M. Berrong, R.M. Weed, and J.M. Young, "Fracture resistance of Kevlar-reinforced
Poly(methyl methacrylate resin: a preliminary study," Int. J. Prosthodont, 3, 391-395, (1990).
13 J. Black, Biological Performence of Materials, Marcel Dekker, New York, (1981).
14 N.R. Boeree, J. Dove, J.J. Cooper, J. Knowles, G. W. Hastings, " Development of a degradable composite for orthopaedic use: mechanical evaluation of a hydroxyapatite-polyhydroxybutyrate composite material," Biomaterials, 14, 793-796 (1993).
15 W. Bonfield, J.C. Behiri, C. Doyle, J. Bowman and J. Abram, "Hydroxyapatite reinforced polyethylene composites for bone replacement," in Biomaterials and Biomechanics 1983, P.Ducheyne, G. van der Perre and A.E. Aubert (eds.) Elsevier Science Publishers B.V., Amsterdam, pp. 421-426, (1984).
16 W. Bonfield, C. Doyle and K. E. Tanner, "In vivo evaluation of hydroxyapatite reinforced polyethylene composites," in Biological and Biomedical Performence of Biomaterials, P.Christel, A. Meunier and A.J.C. Lee (eds.), Elsevier, Amsterdam, pp.153-159, (1986).
Chapter 1 14
17 W. Bonfield, "Composites for bone replacement," J. Biomed.Eng., 10, 522-526, (1988).
18 RL.Bowen, " Properties of a silica-reinforced polymer for dental restoratios.", JADA,66, 71-78, (1963).
19 J.S. Bradley, G.W. Hastings, C. Johnson-Nurse, "carbon-fibre reinforced epoxy as a high strength, low modulus material for internal fixation plates," Biomaterials, 1,38-40, (1980).
20 K.L.B. Brown, R. L. Cruess, "Bone and cartilage transplantation in orthopaedic surgery,"
J. Bone Jt. Surg., 64A, 270-279, (1982).
21 R.A. Casper, B.S. Kelly, R.L. Dunn, A.G. Potter, D.N. Ellis, "Fiber reinforced absorbable composite for orthopaedic surgery," Polym. Mater. Sci. Eng., 53, 497-501 (1985).
22 A. Castaldini, A. Cavallini, A. Moroni, and R. Olmi, "Young's Modulus of hydrxyapatite mixed bone cement," in Biomaterials and Biomechanics 1983, P.Ducheyne, G. van der Perre and A.E. Aubert (eds.) Elsevier Science Publishers B.V., Amsterdam, pp.427-432, (1984).
23 A. Castaldini, A. Cavallini, D. Cavalcoli, " Microstructure and mechanical properties of polymethyl methacrylate composite cements," in Biomaterials and Clinical Applications, A. Pizzoferrato et al (eds.), Elsevier, Amsterdam, pp.517-522, (1987).
24 A. Castaldini, A. Cavallini, "Creep behaviour of composite bone cement," in Biological and Biomedical Performence of Biomaterials, P.Christel, A. Meunier and A.J.C. Lee (eds.), Elsevier, Amsterdam, pp.525-530, (1986).
25 Y.Y. Cheng, O.L. Hui, N.H. Ladizesky, "Processing shrinkage of heat-curing acrylic resin reinforced with high-performence polyethylene fibre," Biomaterilas 14,775-780 (1993).
26 L. Claes, W. Huttner, R. Weiss, "Mechanical properties of carbon fibre reinforced polysulfone plates for intenal fixation," in Biological and Biomechanical Performance of Biomaterials, P. Christel, A. Meunier, and A.J. Lee(eds), Elsvier Sci. , Amsterdam, , 81-86 (1986).
27 D. Coleman, "Mineralization of blood pump bladers," Trans. Am. Soc. Artif. Intern.
Organs, 27:708-713 (1981).
28 A.G.A. Coombes, M.C. Meikle, "Resorbable synthetic polymers as replacement for bone graft," Clin. Mater., 17, 35-67 (1994).
29 E. Dalas, "Crystallization of sparingly soluble salts on functionalized polymers," J. Mater.
Chem., 1, 473-474, (1991a).
30 E. Dalas, J.K. Kallitsis, P. Koutsoukos, "Crystallization of hydroxyapatite on polymers,"
Langmuir, 7, 1822-1826, (1991b).
31 C.J. Damien, J. R. Parsons, "Bone graft and bone graft substitutes: areview of current technology and applications," J. Appl. Biomater., 2, 187-208, (1991).
32 J. Dandurand, V. Delpech, A. Lebugle, A. Lamure, C. Lacabanne, "Study of the
General Introduction 15 mineral-organic linkage in an apatitic reinforced bone cement," J. Biomed. Mater. Res.
24, 1377-1384 (1990).
33 A.U. Daniels, M.K.O. Chang, and K.P. Andriano, "Mechanical properties of Biodegradable polymers and composites proposed for internal fixation of bone," J. Appl.
Biomater. , 1, 57-78, (1990).
34 S. Deb, M. Wang, K.E. Tanner, W. Bonfield, "Hydroxyapatite-polyethylene composites: effect of grafting and surface treatment of hydroxyapatite," J. Mater. Sci. : Mater. in Med. 7, 191-193 (1996).
35 K. de Groot, "Biodegradable ceramics," in Biocompatibility of Implant Materials, D.F.
Williams (ed.), CRC Press, Boca Raton FL. USA, 199-222 (1981)
36 K. de Groot, R.G.T. Geesink, C.P.A.T. Klein, P. Serekian, "Plasma sprayed coatings of hydroxyapatite," J. Biomed. Mater. Res., 21,1375-1378, (1987).
37 H.W. Denissen, H.J.A. van Dijk, K. de Groot, P. J. Klopper, J.P.W. Vermeiden and A.P.
Gehring, "Biological and mechanical evaluation of dense calcium hydroxyapatite made by continuous hot pressing," in Mechanical Properties of Biomaterials, G.W. Hastings, D.F. Williams (eds.), John Willey and Sons, New York, pp. 489-505 (1980).
38 C. Doyle, K.E. Tanner, W. Bonfield, "In vitro and in vivo evaluation of polyhydroxybutyrate and of polyhydroxybutyrate reinforced with hydroxyapatite", Biomaetrials, 12,841-847, (1991).
39 P. Ducheyne, L.L. Hench, I.I.A. Kagan, M. Martens, A. Bursens, J.C. Mulier, "Effect of hydroxyapatite impregnation on skeletal bonding of porous coated implants," J. Biomed.
Mater. Res.14, 225-237, (1980).
40 P. Ducheyne, J.M. Cuckler, "Bioactive ceramic prosthetic coatings," Clin. Orthop. Rl.
Res., 276, 102-114 (1992).
41 A.M.P. Dupraz, J. de Wijn, S.A.T. van der Meer, K. de Groot, "Characterization of silane-treated hydroxyapatite powders for use as filler in biodegradable composites," J. of Biomed. Mater. Res. 30, 231-238,(1996)
42 K. Ekstrand, I.E. Ruyter, H. Wellendorf, "Carbone/graphite fiber reinforced poly(methyl methacrylate): Properties under dry and wet conditions," J. Biomed. Mater.
Res., 21, 1065-1080 (1987).
43 R. Fenner, L. Fambri, C. Migliaresi, "High strength partially absorbable composites produced by sintering method for internal bone fixation," Trans. 5th. World Biomaterials Congress. Toronto. pp. II-440 (1996).
44 K.E. Foy, D. Riddle, Jr., H.D. Schutte, R.A. Latour, Jr., " Interfacial bond hydrolytic stability of calcium phosphate fibers with polycaprolactone polymer," Trans. 5th world Biomaterials Congress, Toronto, I-930 (1996).
45 E.A. Friis, B. Kumar, F.W. Cooke, H.K. Yasuda, "The effect of treated PET additions on the fracture toughness of composite bone cement, " Trans. 5th. World Biomaterials
Chapter 1 16
Congress. Toronto. II-348 (1996).
46 M.L. Gaillard, J. van den Brink, C.A. van Blitterswijk and Z.B. Luklinska, "Applying a calcium phosphate layer on PEO/PBT copolymers affects bone formation in vivo," J.
Mater. Sci. : Mater. in Med., 5, 424-428 (1994).
47 M.L. Gaillard, The Role of Calcium Phosphate in A Bone-bonding Polymer, Ph.D thesis of Leiden University, (1995).
48 J.J. Gilbert, D.S. Ney, E.P. Lautenschlager, "Self-reinforced composite poly(methyl methacrylate): static and fatigue properties," Biomaterails, 16, 1043-1055, (1995.)
49 J. Glowacki, L.B. Kaban, J.E. Murray, J. Folkman, J.B. Mulliken, "Application of the biological principle of induced osteogenesis for craniofacial defects," Lancet, 1,959-963, (1981).
50 G. Guida, V. Riccio, S. Gatto, C. Migliaresi, L. Nicodemo, L. Nicolais, C. Palomba, "A galss bead composite acrylic bone cement," in Biomaterials and Biomechanics 1983, P.Ducheyne, G. van der Perre and A.E. Aubert (eds.) Elsevier Science Publishers B.V., Amsterdam, pp.19-24, (1984).
51 N.L. Hancox, "High performence composites with resin matrices," in Handbook of Composites, Vol 4. Fabrication of Compsites, A. Kelly, S.T. Mileiko (eds.), North Holland, Amsterdam, pp.1-44 (1982).
52 R.S. Hastings, S.A. Brown, A. Moet, "Characterization of short fiber reinforced polymers for fracture fixation device, " Trans. Soc. Biomater. 10, 262 (1987).
53 L.L. Hench, R.J. Splinter, W.C. Allen, T.K. Greenlee, "Bonding mechanism at the interface of ceramic prosthetic materails," J. Biomed. Mater. Res., 2, 117-141 (1971).
54 L.L. Hench, A.E. Clark, " Adhesion to bone," in CRC series in Biocompatibility:
Biocompatibility of Orthopaedic Implants, 2, 129-170 (1981).
55 D.N. Hild, P. Schwartz, "Plasma-treated ultra-high-strength polyethylene fibres improved fracture toughness of poly(methyl methacrylate), " J. Mater. Sci. : Mater. in Med., 4, 481-493 (1993).
56 W. Huettner, G. Keuscher, M. Nietert, "Carbon fiber reinforced polysulfone-thermaoplastic composites," in Biomaterials and Biomechanics, 1983, P.
Ducheyne, G. van der Perre and A.E. Aubert,(eds), Elsevier Science Pub. B.V.
Amsterdam, pp. 167-172 (1984).
57 K. Ishhara, N. Nakabayashi, "Adhesive bone cement both to bone and metals:
4-META in MMA initiated with tri-n-butyl borane", J. Biomed. Mater. Res. 23, 1475-1482, (1989).
58 K. Ishhara, H. Arai, N. Nakabayashi, "Adhesive bone cement containing hydoxyapatite particle as bone compatible filler ," J. Biomed. Mater. Res. 26, 937-945(1992).
59 J. Jancar, A.T. Dibenedetto, "Fibre reinforced thermaoplastic composites for dentistry.
General Introduction 17 Part 1, hydrolytic stability of the interface," J. Mater. Sci.: Mater. in Med., 4, 555-561, (1993).
60 M. Jarcho," Calcium phosphate ceramics as hard tissue prosthetics," Clin. Orthop. Rel.
Res., 157, 259-278 (1981).
61 D.W. Jones, A.S. Rizkalla, "Characterization of experimental composite biomaterials," J.
Biomed. Mater. Res. (Appl. Biomater.), 33, 89-100, (1996).
62 N.L. Jones, D.F. Williams, "Poly(L-lactide) and poly(L-lactide)-ceramic fillered composites: A long term in vivo/in vitro degradation study," Trans. 5th world Biomaterials Congress, Toronto, II-441, (1996).
63 L.B. Kaban, J.B. Mulliken, J. Glowaki, "Treatment of jaw defects with demineralised bone implants," J. Oral Maxillofac., 40, 623-626, (1982).
64 S. Kamei, K. Kato, N. Tomita, S. Tamai, Y. Ikada, "Implantation of hydroxyapatite bonded polymer," Trans. 5th world Biomaterials Congress, Toronto, II-52, (1996).
65 B.S. Kelley, R.L. Dunn, R.A. Casper, "Totally resorbable high-strength composite materials," in Polym. Sci. Technol., Vol. 35, Advances in Biomedical Polymers, C.G.
Gebelein (ed.), Plenum Press, New York, pp.75-85 (1987).
66 B.S. Kelley, R.L. Dunn, T. E. Jacson, A.G. Potter, D.N. Ellis, "Assessment of strength loss in biodegradable composites," Trans. 3rd World Biomaterials Congress, Kyoto, Japan, pp.471, (1988).
67 J.C. Knowles, F.A. Mahmud, and G.W. Hastings, "Piezoelectric charicteristics of a polyhydroxybutyrate based composite", Clinical Mater. 8,155-158 (1991).
68 J.C. Knowles, G.W. Hastings, H. Ohta, S Niwa, N. Boeree, "Development of a degradable composite for orthopaedic use: in vivo biomedical and histological eveluation of two bioactive degradable composites based on the polyhydroxybutyrate polymer,"
Biomaetrials, 13, 491-496, (1992).
69 T. Kokubo, S. Ito, T. Huang, S. Sakka, T. Kitsugi, T. Yamamuro, " Ca, P-rich layer formed on high-strength bioactive glass-ceramic A-W," J. Biomed. Mater. Res., 24 331-343 (1990).
70 T. Kokubo, "Bioactive glass ceramics - properties and applications," Biomaterials, 12, 155-163 (1991).
71 T. Kokubo, H. Kushitani, C. Ohtsuki, S. Sakka, T. Yamamuro, "Effect of ions dissolved from bioactive glass-ceramic on surface apatite formation," J. Mater. Sci.: Mater in Med., 4, 1-4 (1993).
72 W.R. Lacefield, "Hydroxyapatite coatings," in Bioceranics: Material Characteristics versus in vivo Behavior, P. Ducheyne, J.E. Lemons (eds.), The New York Academy of Science, New York, pp.72-78, (1988).
73 J. Laiho, T. Mikkonen, P. Tormala, "A comparison of in vitro degradation of biodegradable polyglycolide (PGA) sutures and rods, " Trans. Soc. Biomater. 11, 564,
Chapter 1 18
74 R.A.. Latour, J. Black, "Development of FRP composite structure biomaterials:Ultimate strength of the fiber/matrix interfacial bond in in vivo simulated environments," J.
Biomed. Mater .Res. , 26, 593,-606(1992).
75 R.A.. Latour, J. Black, "Development of FRP composite structure biomaterials: Fatigue strength of the fiber/matrix inetrfacial bond in simulated in vivo environment, " J.
Biomed. Mater .Res. , 27, 1281-1291,(1993).
76 R.Z. LeGeros, Cacium Phosphates in Oral Biology and Medicine, Karger, Basel, Switzerland, (1991).
77 R. Z. LeGeros, G. Daculsi, I. Orly, M. Gregoire, M. Heughebaert, M. Gineste, R.
kijkowska, "Formation of carbonate apatite on calcium phosphate materials:
dissolution/Precipitation process," in Bone-Bonding Biomaterials, P. Ducheyne, T.
Kokubo, C.A. van Blitterswijk (eds.), Reed Healthcare Communications, pp.201-212 (1992).
78 J.E. Lemons, "Hydroxyapatite coatings," Clin. Orthop., 235, 220-223 (1988).
79 S.H. Li, Q. Liu, J.R. de Wijn, B.L. Zhou, K. de Groot, " Biomimetic coating of bioactive ceramic on bamboo for biomedical application," J. Mater. Sci. Lett., 15, 1882-1885 (1996).
80 S.H. Li, Q. Liu, J.R. de Wijn, B.L. Zhou, K. de Groot, "Calcium phosphate formation induced on silica of bamboo," J. Mater. Sci.: Mater. in Med., (in press) (1997a).
81 S.H. Li, Q. Liu, J.R. de Wijn, B.L. Zhou, K. de Groot, "In vitro calcium phosphate formation on natural composite biomaterial: bamboo," Biomaterials, (in press) (1997b).
82 S.H. Li, Q. Liu, J.R. de Wijn, B.L. Zhou, K. de Groot, "Apatite formation on phosphorylated bamboo," J. Mater. Sci.: Mater. in Med., (in press) (1997c).
83 T.C. Lin, "Totally absorbable fiber reinforced composite for internal fracture fixation devices," Trans. Soc. Biomater., 9, 166 (1986).
84 M. Marcolongo, P. Ducheyne, J. Garino, " Interfacial bond strength between bioactive glass fiber/polymer composite and bone tissue," Trans. Soc. Biomater., 18, 374 (1995).
85 M. Marcolongo, P. Ducheyne, E. Schepers, J. Garino, "The "Halo" effect : surface reactions of a bioactive galss fiber/polymeric composite in vitro and in vivo," Trans. 5th World Biomaterials Congress, Toronto, II-444 (1996).
86 D.N. Misra," Adsorption of zirconyl salts and their acids on hydroxyapatite: use of salts as coupling agents to dental polymer composites," J. Dental Res., 12, 1405-1408 (1985).
87 N. Nishiyama, H. Katsuki, K. Horie, "Adsorbed behavior of spin-labeled silane coupling agent on colloidal silica studied by electron spin resonance," J. Biomed. Mater. Res., 21, 1029-1038 (1987).
88 K. Nishizawa, M. Toriyama, T. Suzuki, Y. Kawamoto, Y. Yokogawa, F. Nagata,
"Surface modification of calcium phosphate ceramics with silane coupling reagents," The
General Introduction 19 Chemical Society of Japan, (in Japaness) 63-67 (1995).
89 S.N. Nazhat, R. Smith., S. Deb, M.Wang, K.E. Tanner, W. Bonfield, "Dynamic mechanical behaviour of modified hydroxyapatite reinforced polyethylene composites,"
Trans. 5th. World Biomaterials Congress, Toronto, pp.II-83 (1996).
90 J.B. Park, R.S. Lakes, Biomaterials: An Introduction, (2nd ed.), Plenum Press, New York, (1992).
91 M. Pellinen, T. Pohjonen, M. Tamminmaki, P, Helevirta, P. Tormala, "The in vitro degradation of biodegradable self-reinforced (SR) polyglycolide rods, " Trans. Soc.
Biomater. 11, 562, (1988).
92 B.J. Perez, H. Alexander, C.W. Mayott, L. Anderson, J.L. Charvet, J. Kohn, W.C.
LaCourse, I. Loh, "Effect of Fiber-Matrix coupling on the mechanical properties of a totally bioabsorbable composite, " Trans. 5th. World Biomaterials Congress, Toronto, II-381 (1996)
93 M.R. Pigott, P.S. Chua, P. Andeison, "The interface between glass and carbon fibers and thermo setting polymers," Polym. Comp., 6, 242-248, (1985).
94 R.M. Pilliar, R. Blackwell, I. MacNab, H. U. Cameron, "Carbon fibre reinforced bone cermnet in orthopaedic surgery", J. Biomed. Mater. Res. 10, 893-906 (1976).
95 E.P. Plueddemann, Silane Coupling Agents, 2nd Edition, Plenum Press, New York, pp.118, (1991).
96 B. Pourdeyhimi, H.D. Wagner, P.A. Schwartz, "A comparison of mechanical properties of discontinuous Kevlar 29 fibre reinforced bone cement", J. Mater. Res. 21, 4468-4474 (1986).
97 D.J. Prolo, J.J. Rodrigo, "Contemporary bone graft physiology and surgery,"
Clin.Orthop., 200, 322-342, (1985).
98 S. Pulapura, C. Li, J. Kohn, "Structure-property relationships for the design of polyiminocarbonates," Biomaterials, 11, 666-678, (1990).
99 S. Pulapura, J. Kohn, "Tyrosine derived polycarbonates: Backbone modified,
"pseudo"-poly(amino acid) designed for biomedical applications," Biopolymers, 32, 411-417 (1992).
100 A. M. Radder, J.E. Davies, R.N.S. Sohdi, S.A.T. va der Meer, J.G.C. Wolke, C.A. van Blitterswijk, " Postoperative carbonate-apatite formation in a polymer matrix:
characterization and relation to bone bonding," Bioceramics 6, 345-351 (1993).
101 A. M. Radder, H. Leenders, C.A. van Blitterswijk, "Interface reaction to PEO/PBT copolymers (Polyactive) after implantation in cortical bone," J. Biomed. Mater. Res., 28, 141-151 (1994).
102 S. Saha, S. Pal, "Mechanical properties of bone cement: a review", J. Biomed. Mater.
Res. 18, 435-462 (1984).
103 F.J. Schoen et al, "Biomaterials associated calcification : pathology, mechanism and
Chapter 1 20
strategies for prevention," J. Biomed. Mater. Res.. 22:11-36 (1988 ).
104 C.K. Schreiber, "Polymethylmethacrylate reinforce with carbon fibres," Br. Dent. J.
105 K. Sinibaldik, H. Rosen, S.-K. Lin, M.De Angelis, "Tumors associated with metallic implants in animals," Clin. Orthop. Rel. Res. , 118, 257-266 (1976).
106 M.A. Slivika, C.C. Chu, I. Adisaputro, "Fiber/matrix interfaces studied on totally and partially absorbable composite materials for internal fixation of bone fractures," Trans.
5th World Biomaterials Congress, Toronto, II-803 (1996).
107 I.A. Small, D. Misiek, "A sixteen-year evaluation of the mandibular staple bone plate," J.
Oral Maxillof. Surg. , 44, 60-67 (1986).
108 U. Soltesz, "Ceramics in composites, review and current status," in Bioceramics:
Materials Characteristics versus in vivo Behavior. P. Ducheyne, J.E. Lemons (eds), Annals of New York Academy of Sciences. Vol. 523, pp.137-156 (1988).
109 D.E. Steflik, A.L. Sisk, G.R. Parr, L.K. Gardner, P.J. Hanes, F.T. Lake, D.J. Berkery and P. Brewer, "Osteogenesis at the dental implant interface: High-voltage electron microscopic and conventional transmission electron microscopic observations," J.
Biomed. Mater. Res., 27, 791-800 (1993).
110 J.N.G. Swart, " Calcification and bone induction studies in heterogenous phosphaorylated hydrogels," in Hydrogels for medical and Related Applications, ACS Symposium Series 31, J.D. Andrade (ed.), pp. 151 (1976).
111 K Tatton, C. Johnson-Nurse, B. Mckibbin, J. Bradley, and G.W. Hastings, "The use of semi-rigid carbon-fibre reinforced plastic plated for fixation of human fractures: results of preliminary trials," J. Bone Jt. Surg. 64B,105-111 (1982).
112 T. Terjesen, K. Apalset, "The influence of different degrees of stiffness of fixation plates on experimental bone healing," J. Orthop. Res., 6, 292-299 (1988).
113 R. J. Thoma, "Poly(ether)urethane reactivity with metal-ion in calcification and enviromental stress cracking," J. Biomater. Appl. , 1:449-486 (1987).
114 L.T.D. Topoleski, P. Ducheyne, "The fracture toughness of titanium-fiber-reinforced bone cerment," J. Biomed. Mater. Res. 26, 1599-1617 (1992).
115 O.N. Tretinnikov, K. Kato, Y. Ikada, "In vitro hydroxyapatite deposition onto a film surface-grafted with organophosphate polymer," J. Biomed. Mater. Res., 28, 1365-1373 (1994).
116 S. Vainionpaa, A. Majola, M. Mero, K. Vihtonen, A. Makela, J. Vasenus, P. Rokkanen, P.
Tormala, "Biodegradation and biocompatibility of the polylactic acid in bone tissue and mechanical properties in vitro, " Trans. Soc. Biomater. 11, 500 (1988).
117 C.A. van Blitterswijk, D. Bakker, H. Leenders, J. v.d.Brink , S.C. Hesseling, Y.P. Bovell, A.M. Radder, R.J. Sakker , M.L. Gallard, P.H. Heinze, G.J. Beumer, "Interfacial reactions leading to bone-bonding with PEO/PBT copolymer (PolyactiveTM)", in
General Introduction 21 Bone-Bonding Biomaterials, P. Ducheyne, T. Kokubo, C.A. van Blitterswijk (eds.), Reed Healthcare Comunications, Leidendorp, the Netherlands, pp.153-171 (1992).
118 C.A. van Blitterswijk, J. v.d.Brink, H. Leenders, D. Bakker, "The effect of PEO ratio on degradation, calcification and bone-bonding of PEO/PBT copolymer(Polyactive)," Cells and Materials, 3, 23-36 (1993).
119 C.A. van Blitterswijk, Y.P. Bovell, J.S. Flash, H. Leenders, I van den Brink, J.D. de Bruijn, "Variation in hydroxyapatite crystalinity: Effects on interface reactions. in Hydroxyapatite Coated Hip and Knee Arthroplasty, edited by J.A. Epinette and R.G.T.
Geesink, Expansion Scientifique Francaise, Paris, pp.33-40 (1995).
120 S.A.T. van der Meer, J. R. de Wijn, J.G.C. Wolke, "The influence of basic filler materials on the degradation of amorphous D- and L-lactide copolymer," J. Mater. Sci.: Mater. In Med., 7, 359-361 (1996).
121 W. van Raemdonck, P. Ducheyne, P. DeMeester, "Auger electron spectroscopic analysis of hydroxyapatite coatings on titanium," J. Am. Ceram. Soc., 6, 381-384, (1984).
122 B.A.M. Venhoven, A.J. de Gee, A. Werner, C.L. Davidson, "Silane treatment of filler and composite blending in a one step procedure for dental restoratives", Biomaterials, 15, 1152-1156 (1994).
123 C.C.P.M. Verheyen, J.R. de Wijn, C.A. van Blitterswijk, K. de Groot,"Evaluation of hydroxyapatite/poly(L-lactide) composites: Mechanical behavior," J. Biomed.
Mater.Res. 26, 1277-1296 (1992).
124 C.C.P.M. Verheyen, J.R. de Wijn, C.A. van Blitterswijk, K. de Groot, P.M. Rozing,
"Hydroxyapatite/poly(L-lactide composites: an animal study on push -out strengths and interface histology," J. Biomed. Mater. Res., 27, 433-444 (1993).
125 M. Wang, D. Porter, W. Bonfield, "Processing, characterisation, and evaluation of hydroxyapatite reinforced polyethylene composites," British Ceramic Transactions, 93, 91-95 (1994).
126 L.M. Wenz, K. Merritt, S.A. Brown, A. Moet, "in vitro biocompatibility of polyetheretherketon and polysulphone composites," J. Biomed. Mater. Res. , 24, 207-215 (1990).
127 D.F. William, A. McNamara, R.M. Turner, "Potential of polyetheretherketon (PEEK) and carbon fibre-reinforced PEEK in medical applications," J. Mater. Sci. Lett., 6,188-190 (1987).
128 D.F. William, J. Black, P.J. Doherty, "Second consensus conference on definitions in biomaterials," in Advances in Biomaterials: Biomaterial-tissue Interfaces 10, P.J. Doherty, R.L. Williams, D.F. Williams and A.J.C. Lee (eds.), Elsevier Science Publishers, Amsterdam, pp.525-533 (1992).
129 C.B. Wisman, W.S. Pierce, J.H. Donachy and W.E. Pae, "A polyurethane trileaflett cardiac valve prosthesis: In vitro and in vivo studies," Trans. Am. Soc. Artif. Intern.
Organs, 28:164-168 (1982).
130 R.T. Wylegala, "Reinforceing denture base material with carbon fibres," Br. Dent.
Chapter 1 22
Technol. 26, 97-100 (1973).
131 M. Zimmerman, J.R. Parsons, H. Alexander, " The design and analysis of a laminated partially degradable composite bone plate for fracture fixation," J. Biomed. Mater. Res.:
Appl. Biomater., 21(A3), 345-361 (1987).
Surface Modification of HA in Polyactive 70/30 Composites 19
Surface Modification of Hydroxyapatite to Introduce Interfacial Bonding With PolyactiveTM
70/30 in A
Qing Liu, Joost R. de Wijn, Dirkjan Bakker# , Clemens A. van Blitterswijk
Biomaterials Research Group, Leiden University , and IBME Research School, Prof. Bronkhorstlaan 10, 3723 MB Bilthoven, # HC Implants bv, Leiden,
A method was developed to improve the interfacial bonding between hydroxyapatite and a biodegradable copolymer PolyactiveTM 70/30. Hydroxyapatite was first surface modified by the polyelectrolytes polyacrylic acid or poly(ethylene-co-maleic acid) in aqueous solutions. Subsequently the surface modified hydroxyapatite was used as filler in composites with PolyactiveTM 70/30. The strength, elongation at break and elastic modulus of the composite in aqueous environment were significantly improved by this method. Based on these experimental results, we believe that the interface improvement is due to the hydrogen bonding and/or dipole interactions formed between polyelectrolyte molecules and polyethylene glycol segments in the polymer matrix. Due to the introduction of interfacial bonding by using such method, a new biodegradable bone-bonding composite can be made.
Chapter 2 20
In recent years, several kinds of polymer-hydroxyapatite composites have been developed as bone substitute materials [1,2,3]. The purpose of making such composites is to reinforce the polymer and improve the bone bonding properties of the material, since it has been found that adding hydroxyapatite (HA) into a polymer matrix may turn an initially non-bioactive polymer into a bone bonding composite, and might simultaneously improve the mechanical properties [1,2,3], especially the elastic modulus and hardness.
In making HA/polymer composites, the lack of interfacial bonding between HA and the polymer matrix still remains an issue of concern [3,4]. The interfacial bonding between inorganic and organic phase plays an important role in determining the ultimate mechanical properties of the composites. A strong interfacial bonding between the two phases usually is necessary for the composites to achieve better mechanical properties. For example, bone, a natural biocomposite, is mainly composed of inorganic bone mineral (hydroxyapatite-like material), organic matrix of type I collagen and noncollagenous proteins . Bone mineral is not directly bound to collagen, but bound to collagen by these non-collagenous proteins . These interfacial bonding forces are mainly ionic bonds, hydrogen bonds and hydrophobic interactions . They give bone unique composite behaviour.
The polymer, PolyactiveTM, used in this study is a block copolymer from polyethylene glycol (PEG) and poly(butylene terephthalate) (PBT). When the weight ratio of PEG/PBT is 55/45 or higher ( the molecular weight of PEG is 1000 Dalton), it is a biodegradable polymer and calcifies postoperatively , thereby inducing bone bonding [7,8]. PolyactiveTM has been already used in making composites with HA. Such composites showed promising results in guided tissue regeneration applications .
However, due to the larger amount of PEG present in the structure of PolyactiveTM 70/30, it is a rubber like polymer with low elastic modulus. In an effort to strengthen the polymer, we chose HA as filler to make HA/polymer composites.
Since in contrast to bone mineral and its collagen matrix, there are no strong bonding forces between HA and PolyactiveTM, it is necessary to introduce some kind of interaction between the two phases by surface modification of HA Such an approach mimics the role of non-collagenous protein in bone.
In this study, a method was developed to improve the interface between HA and PolyactiveTM by using water soluble polyelectrolytes such as polyacrylic acid and poly(ethylene-co-maleic acid). This was based on the principle that polyacrylic acid and the copolymer of maleic acid have the ability to both form complexes with PEG , and be firmly adsorbed onto the surface of HA [11,12].